#------------------------------------------------------------------------------
#$Date: 2016-03-26 16:01:19 +0100 (Sat 26 de Mar de 2016) $
#$Revision: 180368 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/37/7203767.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7203767
loop_
_publ_author_name
'León-Reina, Laura'
'Losilla, Enrique R.'
'Martínez-Lara, Maria'
'Bruque, Sebastián'
'Llobet, Anna'
'Sheptyakov, Denis V.'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Interstitial oxygen in oxygen-stoichiometric apatites
;
_journal_issue                   25
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2489
_journal_paper_doi               10.1039/b503374h
_journal_volume                  15
_journal_year                    2005
_chemical_formula_sum            'La1.33 O4.33 Si Sr0.33'
_chemical_formula_weight         311.83
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.7347(7)
_cell_length_b                   9.7347
_cell_length_c                   7.2531(6)
_cell_volume                     595.25(7)
_computing_structure_refinement  GSAS
_pd_block_id
2004-06-11T10:45|LA8SR2SI6_phase1|La8Sr2Si6O26_750K||
_pd_phase_name
'from C:/RIETVELD/Apatito/SINQ_02/La9.55Si/La955Si6_RT/LA955SI.EXP'
_pd_proc_ls_prof_R_factor        0.0190
_pd_proc_ls_prof_wR_factor       0.0275
_refine_ls_goodness_of_fit_all   1.11
_refine_ls_matrix_type           full
_refine_ls_number_parameters     59
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.07
_refine_ls_shift/su_mean         0.00
_cod_data_source_file            b503374h.txt
_cod_data_source_block           LA8SR2SI6_overall
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (817
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (180 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        595.25037
_cod_database_code               7203767
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.23162(14) -0.01341(15) 0.25 0.8 Uani 0.00692 6
LA La2 0.3333 0.6667 -0.00026(20) 0.8 Uani 0.01206 4
SI SI 0.39992(24) 0.37009(22) 0.25 1.0 Uani 0.00517 6
O O1 0.32340(20) 0.48470(22) 0.25 1.0 Uani 0.01306 6
O O2 0.59321(17) 0.47134(21) 0.25 1.0 Uani 0.01274 6
O O3 0.34152(17) 0.25453(17) 0.07083(13) 1.0 Uani 0.0164 12
O O4 0.0 0.0 0.25 1.027(11) Uani 0.02117 2
SR Sr1 0.23162(14) -0.01341(15) 0.25 0.2 Uani 0.00692 6
SR Sr2 0.33333 0.66667 -0.00026(20) 0.2 Uani 0.01206 4
O O5 0.007 0.241 0.613 -0.0044(18) Uiso 0.03 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 8.0
SI 6.0
O 26.0
SR 2.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 99.55(6) 5_555 . 3_655 n
O1 La1 O3 148.240(28) 5_555 . 1_555 n
O1 La1 O3 71.98(4) 5_555 . 6_555 n
O1 La1 O3 71.98(4) 5_555 . -3_555 n
O1 La1 O3 148.240(28) 5_555 . -4_556 n
O1 La1 O4 110.30(5) 5_555 . 1_555 n
O1 La1 Sr1 140.30(5) 5_555 . 3_555 n
O1 La1 Sr1 80.30(5) 5_555 . 5_555 n
O1 La1 O5 53.79(4) 5_555 . 4_554 n
O1 La1 O5 91.174(26) 5_555 . 5_555 n
O1 La1 O5 154.988(26) 5_555 . 6_554 n
O1 La1 O5 53.79(4) 5_555 . -1_556 n
O1 La1 O5 91.174(26) 5_555 . -2_556 n
O1 La1 O5 154.988(26) 5_555 . -3_556 n
O2 La1 O3 71.77(5) 3_655 . 1_555 n
O2 La1 O3 84.55(4) 3_655 . 6_555 n
O2 La1 O3 84.55(4) 3_655 . -3_555 n
O2 La1 O3 71.77(5) 3_655 . -4_556 n
O2 La1 O4 150.16(6) 3_655 . 1_555 n
O2 La1 Sr1 120.16(6) 3_655 . 3_555 n
O2 La1 Sr1 179.84550(20) 3_655 . 5_555 n
O2 La1 O5 142.05(4) 3_655 . 4_554 n
O2 La1 O5 89.621(25) 3_655 . 5_555 n
O2 La1 O5 90.95(5) 3_655 . 6_554 n
O2 La1 O5 142.05(4) 3_655 . -1_556 n
O2 La1 O5 89.621(25) 3_655 . -2_556 n
O2 La1 O5 90.95(5) 3_655 . -3_556 n
O3 La1 O3 134.72(6) 1_555 . 6_555 n
O3 La1 O3 76.741(26) 1_555 . -3_555 n
O3 La1 O3 59.56(5) 1_555 . -4_556 n
O3 La1 O4 82.44(4) 1_555 . 1_555 n
O3 La1 Sr1 57.12(4) 1_555 . 3_555 n
O3 La1 Sr1 108.37(4) 1_555 . 5_555 n
O3 La1 O5 115.16(4) 1_555 . 4_554 n
O3 La1 O5 118.59(5) 1_555 . 5_555 n
O3 La1 O5 21.016(29) 1_555 . 6_554 n
O3 La1 O5 145.42(5) 1_555 . -1_556 n
O3 La1 O5 59.032(25) 1_555 . -2_556 n
O3 La1 O5 56.731(34) 1_555 . -3_556 n
O3 La1 O3 139.87(8) 6_555 . -3_555 n
O3 La1 O3 76.741(26) 6_555 . -4_556 n
O3 La1 O4 104.27(4) 6_555 . 1_555 n
O3 La1 Sr1 109.44(4) 6_555 . 3_555 n
O3 La1 Sr1 95.40(5) 6_555 . 5_555 n
O3 La1 O5 107.32(5) 6_555 . 4_554 n
O3 La1 O5 21.054(31) 6_555 . 5_555 n
O3 La1 O5 132.02(5) 6_555 . 6_554 n
O3 La1 O5 62.91(4) 6_555 . -1_556 n
O3 La1 O5 160.90(6) 6_555 . -2_556 n
O3 La1 O5 86.646(33) 6_555 . -3_556 n
O3 La1 O3 134.72(6) -3_555 . -4_556 n
O3 La1 O4 104.27(4) -3_555 . 1_555 n
O3 La1 Sr1 109.44(4) -3_555 . 3_555 n
O3 La1 Sr1 95.40(5) -3_555 . 5_555 n
O3 La1 O5 62.91(4) -3_555 . 4_554 n
O3 La1 O5 160.90(6) -3_555 . 5_555 n
O3 La1 O5 86.646(33) -3_555 . 6_554 n
O3 La1 O5 107.32(5) -3_555 . -1_556 n
O3 La1 O5 21.054(31) -3_555 . -2_556 n
O3 La1 O5 132.02(5) -3_555 . -3_556 n
O3 La1 O4 82.44(4) -4_556 . 1_555 n
O3 La1 Sr1 57.12(4) -4_556 . 3_555 n
O3 La1 Sr1 108.37(4) -4_556 . 5_555 n
O3 La1 O5 145.42(5) -4_556 . 4_554 n
O3 La1 O5 59.032(25) -4_556 . 5_555 n
O3 La1 O5 56.731(34) -4_556 . 6_554 n
O3 La1 O5 115.16(4) -4_556 . -1_556 n
O3 La1 O5 118.59(5) -4_556 . -2_556 n
O3 La1 O5 21.016(29) -4_556 . -3_556 n
O4 La1 Sr1 30.0 1_555 . 3_555 n
O4 La1 Sr1 30.0 1_555 . 5_555 n
O4 La1 O5 63.133(28) 1_555 . 4_554 n
O4 La1 O5 89.768(23) 1_555 . 5_555 n
O4 La1 O5 61.767(26) 1_555 . 6_554 n
O4 La1 O5 63.133(28) 1_555 . -1_556 n
O4 La1 O5 89.768(23) 1_555 . -2_556 n
O4 La1 O5 61.767(26) 1_555 . -3_556 n
Sr1 La1 Sr1 60.0 3_555 . 5_555 n
Sr1 La1 O5 90.406(26) 3_555 . 4_554 n
Sr1 La1 O5 89.216(24) 3_555 . 5_555 n
Sr1 La1 O5 36.361(25) 3_555 . 6_554 n
Sr1 La1 O5 90.406(26) 3_555 . -1_556 n
Sr1 La1 O5 89.216(24) 3_555 . -2_556 n
Sr1 La1 O5 36.361(25) 3_555 . -3_556 n
Sr1 La1 O5 37.829(28) 5_555 . 4_554 n
Sr1 La1 O5 90.382(25) 5_555 . 5_555 n
Sr1 La1 O5 89.195(24) 5_555 . 6_554 n
Sr1 La1 O5 37.829(28) 5_555 . -1_556 n
Sr1 La1 O5 90.382(25) 5_555 . -2_556 n
Sr1 La1 O5 89.195(24) 5_555 . -3_556 n
O5 La1 O5 114.53(4) 4_554 . 5_555 n
O5 La1 O5 105.157(30) 4_554 . 6_554 n
O5 La1 O5 47.262(23) 4_554 . -1_556 n
O5 La1 O5 67.271(16) 4_554 . -2_556 n
O5 La1 O5 124.90(4) 4_554 . -3_556 n
O5 La1 O5 111.68(4) 5_555 . 6_554 n
O5 La1 O5 67.271(16) 5_555 . -1_556 n
O5 La1 O5 177.62(5) 5_555 . -2_556 n
O5 La1 O5 66.083(15) 5_555 . -3_556 n
O5 La1 O5 124.90(4) 6_554 . -1_556 n
O5 La1 O5 66.083(15) 6_554 . -2_556 n
O5 La1 O5 45.596(21) 6_554 . -3_556 n
O5 La1 O5 114.53(4) -1_556 . -2_556 n
O5 La1 O5 105.157(30) -1_556 . -3_556 n
O5 La1 O5 111.68(4) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 136.44(4) -2_565 . 1_555 n
La2 La2 O1 136.45(4) -2_565 . 3_665 n
La2 La2 O1 136.48(4) -2_565 . 5_565 n
La2 La2 O2 44.99(4) -2_565 . 2_554 n
La2 La2 O2 44.98(4) -2_565 . 4_664 n
La2 La2 O2 44.98(4) -2_565 . 6_564 n
La2 La2 Sr2 89.9756 -2_565 . 1_555 n
La2 La2 Sr2 0.0 -2_565 . -2_565 n
La2 La2 Sr2 179.972 -2_565 . -2_566 n
La2 La2 O1 43.54(4) -2_566 . 1_555 n
La2 La2 O1 43.53(4) -2_566 . 3_665 n
La2 La2 O1 43.55(4) -2_566 . 5_565 n
La2 La2 O2 135.04(4) -2_566 . 2_554 n
La2 La2 O2 135.00(4) -2_566 . 4_664 n
La2 La2 O2 135.02(4) -2_566 . 6_564 n
La2 La2 Sr2 90.000(35) -2_566 . 1_555 n
La2 La2 Sr2 179.972 -2_566 . -2_565 n
La2 La2 Sr2 0.0 -2_566 . -2_566 n
O1 La2 O1 73.25(6) 1_555 . 3_665 n
O1 La2 O1 73.25(6) 1_555 . 5_565 n
O1 La2 O2 125.02(4) 1_555 . 2_554 n
O1 La2 O2 93.64(4) 1_555 . 4_664 n
O1 La2 O2 154.21(5) 1_555 . 6_564 n
O1 La2 Sr2 54.5831 1_555 . 1_555 n
O1 La2 Sr2 136.44(4) 1_555 . -2_565 n
O1 La2 Sr2 43.54(4) 1_555 . -2_566 n
O1 La2 O1 73.26(6) 3_665 . 5_565 n
O1 La2 O2 154.25(5) 3_665 . 2_554 n
O1 La2 O2 125.00(4) 3_665 . 4_664 n
O1 La2 O2 93.66(4) 3_665 . 6_564 n
O1 La2 Sr2 88.079(32) 3_665 . 1_555 n
O1 La2 Sr2 136.46(4) 3_665 . -2_565 n
O1 La2 Sr2 43.54(4) 3_665 . -2_566 n
O1 La2 O2 93.67(4) 5_565 . 2_554 n
O1 La2 O2 154.22(5) 5_565 . 4_664 n
O1 La2 O2 125.04(4) 5_565 . 6_564 n
O1 La2 Sr2 127.740(30) 5_565 . 1_555 n
O1 La2 Sr2 136.47(4) 5_565 . -2_565 n
O1 La2 Sr2 43.54(4) 5_565 . -2_566 n
O2 La2 O2 75.49(6) 2_554 . 4_664 n
O2 La2 O2 75.50(6) 2_554 . 6_564 n
O2 La2 Sr2 116.99(4) 2_554 . 1_555 n
O2 La2 Sr2 44.98(4) 2_554 . -2_565 n
O2 La2 Sr2 135.03(4) 2_554 . -2_566 n
O2 La2 O2 75.49(6) 4_664 . 6_564 n
O2 La2 Sr2 45.87(4) 4_664 . 1_555 n
O2 La2 Sr2 44.98(4) 4_664 . -2_565 n
O2 La2 Sr2 135.00(4) 4_664 . -2_566 n
O2 La2 Sr2 103.977(23) 6_564 . 1_555 n
O2 La2 Sr2 44.98(4) 6_564 . -2_565 n
O2 La2 Sr2 135.02(4) 6_564 . -2_566 n
Sr2 La2 Sr2 89.9956 1_555 . -2_565 n
Sr2 La2 Sr2 90.020(17) 1_555 . -2_566 n
Sr2 La2 Sr2 180.0 -2_565 . -2_566 n
O1 SI O2 111.86(15) 1_555 . 1_555 n
O1 SI O3 110.75(10) 1_555 . 1_555 n
O1 SI O3 110.75(10) 1_555 . -4_556 n
O1 SI Sr1 130.60(12) 1_555 . 1_555 n
O1 SI Sr1 55.05(9) 1_555 . 3_555 n
O1 SI Sr2 136.48(8) 1_555 . 2_655 n
O1 SI Sr2 136.48(8) 1_555 . -1_665 n
O1 SI O5 89.12(10) 1_555 . 6_554 n
O1 SI O5 89.12(10) 1_555 . -3_556 n
O2 SI O3 108.50(10) 1_555 . 1_555 n
O2 SI O3 108.50(10) 1_555 . -4_556 n
O2 SI Sr1 117.54(11) 1_555 . 1_555 n
O2 SI Sr1 166.91(12) 1_555 . 3_555 n
O2 SI Sr2 48.58(6) 1_555 . 2_655 n
O2 SI Sr2 48.58(6) 1_555 . -1_665 n
O2 SI O5 140.44(7) 1_555 . 6_554 n
O2 SI O5 140.44(7) 1_555 . -3_556 n
O3 SI O3 106.28(14) 1_555 . -4_556 n
O3 SI Sr1 53.27(7) 1_555 . 1_555 n
O3 SI Sr1 78.83(8) 1_555 . 3_555 n
O3 SI Sr2 112.50(10) 1_555 . 2_655 n
O3 SI Sr2 60.78(7) 1_555 . -1_665 n
O3 SI O5 32.20(6) 1_555 . 6_554 n
O3 SI O5 93.38(11) 1_555 . -3_556 n
O3 SI Sr1 53.27(7) -4_556 . 1_555 n
O3 SI Sr1 78.83(8) -4_556 . 3_555 n
O3 SI Sr2 60.78(7) -4_556 . 2_655 n
O3 SI Sr2 112.50(10) -4_556 . -1_665 n
O3 SI O5 93.38(11) -4_556 . 6_554 n
O3 SI O5 32.20(6) -4_556 . -3_556 n
Sr1 SI Sr1 75.55(5) 1_555 . 3_555 n
Sr1 SI Sr2 81.28(4) 1_555 . 2_655 n
Sr1 SI Sr2 81.28(4) 1_555 . -1_665 n
Sr1 SI O5 51.98(5) 1_555 . 6_554 n
Sr1 SI O5 51.98(5) 1_555 . -3_556 n
Sr1 SI Sr2 139.58(4) 3_555 . 2_655 n
Sr1 SI Sr2 139.58(4) 3_555 . -1_665 n
Sr1 SI O5 46.79(5) 3_555 . 6_554 n
Sr1 SI O5 46.79(5) 3_555 . -3_556 n
Sr2 SI Sr2 65.93(6) 2_655 . -1_665 n
Sr2 SI O5 131.83(9) 2_655 . 6_554 n
Sr2 SI O5 92.94(5) 2_655 . -3_556 n
Sr2 SI O5 92.94(5) -1_665 . 6_554 n
Sr2 SI O5 131.83(9) -1_665 . -3_556 n
O5 SI O5 68.89(7) 6_554 . -3_556 n
La1 O1 La2 103.82(5) 3_555 . 1_555 n
La1 O1 La2 103.83(5) 3_555 . -2_566 n
La1 O1 SI 95.93(11) 3_555 . 1_555 n
La1 O1 Sr1 0.0 3_555 . 3_555 n
La1 O1 Sr2 103.82(5) 3_555 . 1_555 n
La1 O1 Sr2 103.82(5) 3_555 . -2_566 n
La2 O1 La2 92.91(7) 1_555 . -2_566 n
La2 O1 SI 128.18(5) 1_555 . 1_555 n
La2 O1 Sr1 103.82(5) 1_555 . 3_555 n
La2 O1 Sr2 0.0 1_555 . 1_555 n
La2 O1 Sr2 92.91(7) 1_555 . -2_566 n
La2 O1 SI 128.16(5) -2_566 . 1_555 n
La2 O1 Sr1 103.83(5) -2_566 . 3_555 n
La2 O1 Sr2 92.92(7) -2_566 . 1_555 n
La2 O1 Sr2 0.0 -2_566 . -2_566 n
SI O1 Sr1 95.93(11) 1_555 . 3_555 n
SI O1 Sr2 128.17(5) 1_555 . 1_555 n
SI O1 Sr2 128.17(5) 1_555 . -2_566 n
Sr1 O1 Sr2 103.82(5) 3_555 . 1_555 n
Sr1 O1 Sr2 103.82(5) 3_555 . -2_566 n
Sr2 O1 Sr2 92.92(7) 1_555 . -2_566 n
La1 O2 La2 115.22(5) 5_665 . 2_655 n
La1 O2 La2 115.21(5) 5_665 . -1_665 n
La1 O2 SI 124.52(12) 5_665 . 1_555 n
La1 O2 Sr1 0.0 5_665 . 5_665 n
La1 O2 Sr2 115.21(5) 5_665 . 2_655 n
La1 O2 Sr2 115.21(5) 5_665 . -1_665 n
La2 O2 La2 90.03(8) 2_655 . -1_665 n
La2 O2 SI 102.90(7) 2_655 . 1_555 n
La2 O2 Sr1 115.22(5) 2_655 . 5_665 n
La2 O2 Sr2 0.0 2_655 . 2_655 n
La2 O2 Sr2 90.04(8) 2_655 . -1_665 n
La2 O2 SI 102.91(7) -1_665 . 1_555 n
La2 O2 Sr1 115.21(5) -1_665 . 5_665 n
La2 O2 Sr2 90.03(8) -1_665 . 2_655 n
La2 O2 Sr2 0.0 -1_665 . -1_665 n
SI O2 Sr1 124.52(12) 1_555 . 5_665 n
SI O2 Sr2 102.91(7) 1_555 . 2_655 n
SI O2 Sr2 102.91(7) 1_555 . -1_665 n
Sr1 O2 Sr2 115.21(5) 5_665 . 2_655 n
Sr1 O2 Sr2 115.21(5) 5_665 . -1_665 n
Sr2 O2 Sr2 90.04(8) 2_655 . -1_665 n
La1 O3 La1 115.41(7) 1_555 . 2_554 n
La1 O3 SI 96.90(7) 1_555 . 1_555 n
La1 O3 Sr1 0.0 1_555 . 1_555 n
La1 O3 Sr1 115.41(7) 1_555 . 2_554 n
La1 O3 Sr2 101.49(4) 1_555 . -1_665 n
La1 O3 O5 76.39(8) 1_555 . 6_554 n
La1 O3 SI 143.09(9) 2_554 . 1_555 n
La1 O3 Sr1 115.41(7) 2_554 . 1_555 n
La1 O3 Sr1 0.0 2_554 . 2_554 n
La1 O3 Sr2 99.92(5) 2_554 . -1_665 n
La1 O3 O5 88.80(7) 2_554 . 6_554 n
SI O3 Sr1 96.90(7) 1_555 . 1_555 n
SI O3 Sr1 143.09(9) 1_555 . 2_554 n
SI O3 Sr2 90.01(9) 1_555 . -1_665 n
SI O3 O5 81.64(10) 1_555 . 6_554 n
Sr1 O3 Sr1 115.41(7) 1_555 . 2_554 n
Sr1 O3 Sr2 101.49(4) 1_555 . -1_665 n
Sr1 O3 O5 76.39(8) 1_555 . 6_554 n
Sr1 O3 Sr2 99.92(5) 2_554 . -1_665 n
Sr1 O3 O5 88.80(7) 2_554 . 6_554 n
Sr2 O3 O5 171.01(8) -1_665 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 Sr1 0.0 1_555 . 1_555 n
La1 O4 Sr1 120.0 1_555 . 3_555 n
La1 O4 Sr1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 3_555 . 1_555 n
La1 O4 Sr1 0.0 3_555 . 3_555 n
La1 O4 Sr1 120.0 3_555 . 5_555 n
La1 O4 Sr1 120.0 5_555 . 1_555 n
La1 O4 Sr1 120.0 5_555 . 3_555 n
La1 O4 Sr1 0.0 5_555 . 5_555 n
Sr1 O4 Sr1 120.0 1_555 . 3_555 n
Sr1 O4 Sr1 120.0 1_555 . 5_555 n
Sr1 O4 Sr1 120.0 3_555 . 5_555 n
La1 Sr1 La1 60.0 3_555 . 5_555 n
La1 Sr1 SI 53.17(5) 3_555 . 1_555 n
La1 Sr1 SI 111.27(5) 3_555 . 5_555 n
La1 Sr1 O1 140.30(5) 3_555 . 5_555 n
La1 Sr1 O2 120.16(6) 3_555 . 3_655 n
La1 Sr1 O3 57.12(4) 3_555 . 1_555 n
La1 Sr1 O3 109.44(4) 3_555 . 6_555 n
La1 Sr1 O3 109.44(4) 3_555 . -3_555 n
La1 Sr1 O3 57.12(4) 3_555 . -4_556 n
La1 Sr1 O4 30.0 3_555 . 1_555 n
La1 Sr1 Sr1 0.0 3_555 . 3_555 n
La1 Sr1 Sr1 60.0 3_555 . 5_555 n
La1 Sr1 Sr2 150.709(23) 3_555 . 1_545 n
La1 Sr1 Sr2 97.50(4) 3_555 . 2_655 n
La1 Sr1 Sr2 97.50(4) 3_555 . -1_665 n
La1 Sr1 Sr2 150.709(23) 3_555 . -2_556 n
La1 Sr1 O5 90.406(26) 3_555 . 4_554 n
La1 Sr1 O5 89.216(24) 3_555 . 5_555 n
La1 Sr1 O5 36.361(25) 3_555 . 6_554 n
La1 Sr1 O5 90.406(26) 3_555 . -1_556 n
La1 Sr1 O5 89.216(24) 3_555 . -2_556 n
La1 Sr1 O5 36.361(25) 3_555 . -3_556 n
La1 Sr1 SI 113.17(5) 5_555 . 1_555 n
La1 Sr1 SI 51.27(5) 5_555 . 5_555 n
La1 Sr1 O1 80.30(5) 5_555 . 5_555 n
La1 Sr1 O2 179.84550(20) 5_555 . 3_655 n
La1 Sr1 O3 108.37(4) 5_555 . 1_555 n
La1 Sr1 O3 95.40(5) 5_555 . 6_555 n
La1 Sr1 O3 95.40(5) 5_555 . -3_555 n
La1 Sr1 O3 108.37(4) 5_555 . -4_556 n
La1 Sr1 O4 30.0 5_555 . 1_555 n
La1 Sr1 Sr1 60.0 5_555 . 3_555 n
La1 Sr1 Sr1 0.0 5_555 . 5_555 n
La1 Sr1 Sr2 104.47(4) 5_555 . 1_545 n
La1 Sr1 Sr2 147.318(26) 5_555 . 2_655 n
La1 Sr1 Sr2 147.318(26) 5_555 . -1_665 n
La1 Sr1 Sr2 104.47(4) 5_555 . -2_556 n
La1 Sr1 O5 37.829(28) 5_555 . 4_554 n
La1 Sr1 O5 90.382(25) 5_555 . 5_555 n
La1 Sr1 O5 89.195(24) 5_555 . 6_554 n
La1 Sr1 O5 37.829(28) 5_555 . -1_556 n
La1 Sr1 O5 90.382(25) 5_555 . -2_556 n
La1 Sr1 O5 89.195(24) 5_555 . -3_556 n
SI Sr1 SI 164.45(5) 1_555 . 5_555 n
SI Sr1 O1 166.53(6) 1_555 . 5_555 n
SI Sr1 O2 66.98(6) 1_555 . 3_655 n
SI Sr1 O3 29.834(27) 1_555 . 1_555 n
SI Sr1 O3 105.44(4) 1_555 . 6_555 n
SI Sr1 O3 105.44(4) 1_555 . -3_555 n
SI Sr1 O3 29.834(27) 1_555 . -4_556 n
SI Sr1 O4 83.17(5) 1_555 . 1_555 n
SI Sr1 Sr1 53.17(5) 1_555 . 3_555 n
SI Sr1 Sr1 113.17(5) 1_555 . 5_555 n
SI Sr1 Sr2 134.02(4) 1_555 . 1_545 n
SI Sr1 Sr2 50.250(34) 1_555 . 2_655 n
SI Sr1 Sr2 50.250(34) 1_555 . -1_665 n
SI Sr1 Sr2 134.01(4) 1_555 . -2_556 n
SI Sr1 O5 137.52(4) 1_555 . 4_554 n
SI Sr1 O5 88.815(27) 1_555 . 5_555 n
SI Sr1 O5 32.660(29) 1_555 . 6_554 n
SI Sr1 O5 137.52(4) 1_555 . -1_556 n
SI Sr1 O5 88.815(27) 1_555 . -2_556 n
SI Sr1 O5 32.660(29) 1_555 . -3_556 n
SI Sr1 O1 29.02(5) 5_555 . 5_555 n
SI Sr1 O2 128.57(6) 5_555 . 3_655 n
SI Sr1 O3 145.90(4) 5_555 . 1_555 n
SI Sr1 O3 78.55(4) 5_555 . 6_555 n
SI Sr1 O3 78.55(4) 5_555 . -3_555 n
SI Sr1 O3 145.90(4) 5_555 . -4_556 n
SI Sr1 O4 81.27(5) 5_555 . 1_555 n
SI Sr1 Sr1 111.27(5) 5_555 . 3_555 n
SI Sr1 Sr1 51.27(5) 5_555 . 5_555 n
SI Sr1 Sr2 58.885(33) 5_555 . 1_545 n
SI Sr1 Sr2 142.01(4) 5_555 . 2_655 n
SI Sr1 Sr2 142.01(4) 5_555 . -1_665 n
SI Sr1 Sr2 58.886(33) 5_555 . -2_556 n
SI Sr1 O5 31.100(25) 5_555 . 4_554 n
SI Sr1 O5 91.117(27) 5_555 . 5_555 n
SI Sr1 O5 135.26(5) 5_555 . 6_554 n
SI Sr1 O5 31.100(25) 5_555 . -1_556 n
SI Sr1 O5 91.117(27) 5_555 . -2_556 n
SI Sr1 O5 135.26(5) 5_555 . -3_556 n
O1 Sr1 O2 99.55(6) 5_555 . 3_655 n
O1 Sr1 O3 148.240(28) 5_555 . 1_555 n
O1 Sr1 O3 71.98(4) 5_555 . 6_555 n
O1 Sr1 O3 71.98(4) 5_555 . -3_555 n
O1 Sr1 O3 148.240(28) 5_555 . -4_556 n
O1 Sr1 O4 110.30(5) 5_555 . 1_555 n
O1 Sr1 Sr1 140.30(5) 5_555 . 3_555 n
O1 Sr1 Sr1 80.30(5) 5_555 . 5_555 n
O1 Sr1 Sr2 36.068(26) 5_555 . 1_545 n
O1 Sr1 Sr2 118.19(4) 5_555 . 2_655 n
O1 Sr1 Sr2 118.19(4) 5_555 . -1_665 n
O1 Sr1 Sr2 36.068(26) 5_555 . -2_556 n
O1 Sr1 O5 53.79(4) 5_555 . 4_554 n
O1 Sr1 O5 91.174(26) 5_555 . 5_555 n
O1 Sr1 O5 154.988(26) 5_555 . 6_554 n
O1 Sr1 O5 53.79(4) 5_555 . -1_556 n
O1 Sr1 O5 91.174(26) 5_555 . -2_556 n
O1 Sr1 O5 154.988(26) 5_555 . -3_556 n
O2 Sr1 O3 71.77(5) 3_655 . 1_555 n
O2 Sr1 O3 84.55(4) 3_655 . 6_555 n
O2 Sr1 O3 84.55(4) 3_655 . -3_555 n
O2 Sr1 O3 71.77(5) 3_655 . -4_556 n
O2 Sr1 O4 150.16(6) 3_655 . 1_555 n
O2 Sr1 Sr1 120.16(6) 3_655 . 3_555 n
O2 Sr1 Sr1 179.84550(20) 3_655 . 5_555 n
O2 Sr1 Sr2 75.39(4) 3_655 . 1_545 n
O2 Sr1 Sr2 32.780(28) 3_655 . 2_655 n
O2 Sr1 Sr2 32.779(28) 3_655 . -1_665 n
O2 Sr1 Sr2 75.39(4) 3_655 . -2_556 n
O2 Sr1 O5 142.05(4) 3_655 . 4_554 n
O2 Sr1 O5 89.621(25) 3_655 . 5_555 n
O2 Sr1 O5 90.95(5) 3_655 . 6_554 n
O2 Sr1 O5 142.05(4) 3_655 . -1_556 n
O2 Sr1 O5 89.621(25) 3_655 . -2_556 n
O2 Sr1 O5 90.95(5) 3_655 . -3_556 n
O3 Sr1 O3 134.72(6) 1_555 . 6_555 n
O3 Sr1 O3 76.741(26) 1_555 . -3_555 n
O3 Sr1 O3 59.56(5) 1_555 . -4_556 n
O3 Sr1 O4 82.44(4) 1_555 . 1_555 n
O3 Sr1 Sr1 57.12(4) 1_555 . 3_555 n
O3 Sr1 Sr1 108.37(4) 1_555 . 5_555 n
O3 Sr1 Sr2 113.623(32) 1_555 . 1_545 n
O3 Sr1 Sr2 70.97(4) 1_555 . 2_655 n
O3 Sr1 Sr2 41.704(33) 1_555 . -1_665 n
O3 Sr1 Sr2 146.85(5) 1_555 . -2_556 n
O3 Sr1 O5 115.16(4) 1_555 . 4_554 n
O3 Sr1 O5 118.59(5) 1_555 . 5_555 n
O3 Sr1 O5 21.016(29) 1_555 . 6_554 n
O3 Sr1 O5 145.42(5) 1_555 . -1_556 n
O3 Sr1 O5 59.032(25) 1_555 . -2_556 n
O3 Sr1 O5 56.731(34) 1_555 . -3_556 n
O3 Sr1 O3 139.87(8) 6_555 . -3_555 n
O3 Sr1 O3 76.741(26) 6_555 . -4_556 n
O3 Sr1 O4 104.27(4) 6_555 . 1_555 n
O3 Sr1 Sr1 109.44(4) 6_555 . 3_555 n
O3 Sr1 Sr1 95.40(5) 6_555 . 5_555 n
O3 Sr1 Sr2 96.01(5) 6_555 . 1_545 n
O3 Sr1 Sr2 68.52(4) 6_555 . 2_655 n
O3 Sr1 Sr2 115.40(5) 6_555 . -1_665 n
O3 Sr1 Sr2 43.86(4) 6_555 . -2_556 n
O3 Sr1 O5 107.32(5) 6_555 . 4_554 n
O3 Sr1 O5 21.054(31) 6_555 . 5_555 n
O3 Sr1 O5 132.02(5) 6_555 . 6_554 n
O3 Sr1 O5 62.91(4) 6_555 . -1_556 n
O3 Sr1 O5 160.90(6) 6_555 . -2_556 n
O3 Sr1 O5 86.646(33) 6_555 . -3_556 n
O3 Sr1 O3 134.72(6) -3_555 . -4_556 n
O3 Sr1 O4 104.27(4) -3_555 . 1_555 n
O3 Sr1 Sr1 109.44(4) -3_555 . 3_555 n
O3 Sr1 Sr1 95.40(5) -3_555 . 5_555 n
O3 Sr1 Sr2 43.86(4) -3_555 . 1_545 n
O3 Sr1 Sr2 115.40(5) -3_555 . 2_655 n
O3 Sr1 Sr2 68.52(4) -3_555 . -1_665 n
O3 Sr1 Sr2 96.01(5) -3_555 . -2_556 n
O3 Sr1 O5 62.91(4) -3_555 . 4_554 n
O3 Sr1 O5 160.90(6) -3_555 . 5_555 n
O3 Sr1 O5 86.646(33) -3_555 . 6_554 n
O3 Sr1 O5 107.32(5) -3_555 . -1_556 n
O3 Sr1 O5 21.054(31) -3_555 . -2_556 n
O3 Sr1 O5 132.02(5) -3_555 . -3_556 n
O3 Sr1 O4 82.44(4) -4_556 . 1_555 n
O3 Sr1 Sr1 57.12(4) -4_556 . 3_555 n
O3 Sr1 Sr1 108.37(4) -4_556 . 5_555 n
O3 Sr1 Sr2 146.86(5) -4_556 . 1_545 n
O3 Sr1 Sr2 41.704(33) -4_556 . 2_655 n
O3 Sr1 Sr2 70.97(4) -4_556 . -1_665 n
O3 Sr1 Sr2 113.623(32) -4_556 . -2_556 n
O3 Sr1 O5 145.42(5) -4_556 . 4_554 n
O3 Sr1 O5 59.032(25) -4_556 . 5_555 n
O3 Sr1 O5 56.731(34) -4_556 . 6_554 n
O3 Sr1 O5 115.16(4) -4_556 . -1_556 n
O3 Sr1 O5 118.59(5) -4_556 . -2_556 n
O3 Sr1 O5 21.016(29) -4_556 . -3_556 n
O4 Sr1 Sr1 30.0 1_555 . 3_555 n
O4 Sr1 Sr1 30.0 1_555 . 5_555 n
O4 Sr1 Sr2 130.38(4) 1_555 . 1_545 n
O4 Sr1 Sr2 124.14(4) 1_555 . 2_655 n
O4 Sr1 Sr2 124.14(4) 1_555 . -1_665 n
O4 Sr1 Sr2 130.38(4) 1_555 . -2_556 n
O4 Sr1 O5 63.133(28) 1_555 . 4_554 n
O4 Sr1 O5 89.768(23) 1_555 . 5_555 n
O4 Sr1 O5 61.767(26) 1_555 . 6_554 n
O4 Sr1 O5 63.133(28) 1_555 . -1_556 n
O4 Sr1 O5 89.768(23) 1_555 . -2_556 n
O4 Sr1 O5 61.767(26) 1_555 . -3_556 n
Sr1 Sr1 Sr1 60.0 3_555 . 5_555 n
Sr1 Sr1 Sr2 150.709(23) 3_555 . 1_545 n
Sr1 Sr1 Sr2 97.50(4) 3_555 . 2_655 n
Sr1 Sr1 Sr2 97.50(4) 3_555 . -1_665 n
Sr1 Sr1 Sr2 150.709(23) 3_555 . -2_556 n
Sr1 Sr1 O5 90.406(26) 3_555 . 4_554 n
Sr1 Sr1 O5 89.216(24) 3_555 . 5_555 n
Sr1 Sr1 O5 36.361(25) 3_555 . 6_554 n
Sr1 Sr1 O5 90.406(26) 3_555 . -1_556 n
Sr1 Sr1 O5 89.216(24) 3_555 . -2_556 n
Sr1 Sr1 O5 36.361(25) 3_555 . -3_556 n
Sr1 Sr1 Sr2 104.47(4) 5_555 . 1_545 n
Sr1 Sr1 Sr2 147.318(26) 5_555 . 2_655 n
Sr1 Sr1 Sr2 147.318(26) 5_555 . -1_665 n
Sr1 Sr1 Sr2 104.47(4) 5_555 . -2_556 n
Sr1 Sr1 O5 37.829(28) 5_555 . 4_554 n
Sr1 Sr1 O5 90.382(25) 5_555 . 5_555 n
Sr1 Sr1 O5 89.195(24) 5_555 . 6_554 n
Sr1 Sr1 O5 37.829(28) 5_555 . -1_556 n
Sr1 Sr1 O5 90.382(25) 5_555 . -2_556 n
Sr1 Sr1 O5 89.195(24) 5_555 . -3_556 n
Sr2 Sr1 Sr2 105.365(24) 1_545 . 2_655 n
Sr2 Sr1 Sr2 83.853(16) 1_545 . -1_665 n
Sr2 Sr1 Sr2 52.14(4) 1_545 . -2_556 n
Sr2 Sr1 O5 67.711(23) 1_545 . 4_554 n
Sr2 Sr1 O5 117.04(4) 1_545 . 5_555 n
Sr2 Sr1 O5 128.940(22) 1_545 . 6_554 n
Sr2 Sr1 O5 88.456(34) 1_545 . -1_556 n
Sr2 Sr1 O5 64.906(25) 1_545 . -2_556 n
Sr2 Sr1 O5 165.72(4) 1_545 . -3_556 n
Sr2 Sr1 Sr2 50.08(4) 2_655 . -1_665 n
Sr2 Sr1 Sr2 83.853(16) 2_655 . -2_556 n
Sr2 Sr1 O5 171.93(4) 2_655 . 4_554 n
Sr2 Sr1 O5 64.191(25) 2_655 . 5_555 n
Sr2 Sr1 O5 82.343(32) 2_655 . 6_554 n
Sr2 Sr1 O5 130.600(20) 2_655 . -1_556 n
Sr2 Sr1 O5 114.27(4) 2_655 . -2_556 n
Sr2 Sr1 O5 62.532(22) 2_655 . -3_556 n
Sr2 Sr1 Sr2 105.365(24) -1_665 . -2_556 n
Sr2 Sr1 O5 130.600(20) -1_665 . 4_554 n
Sr2 Sr1 O5 114.27(4) -1_665 . 5_555 n
Sr2 Sr1 O5 62.532(22) -1_665 . 6_554 n
Sr2 Sr1 O5 171.93(4) -1_665 . -1_556 n
Sr2 Sr1 O5 64.191(25) -1_665 . -2_556 n
Sr2 Sr1 O5 82.343(32) -1_665 . -3_556 n
Sr2 Sr1 O5 88.456(34) -2_556 . 4_554 n
Sr2 Sr1 O5 64.906(25) -2_556 . 5_555 n
Sr2 Sr1 O5 165.72(4) -2_556 . 6_554 n
Sr2 Sr1 O5 67.711(23) -2_556 . -1_556 n
Sr2 Sr1 O5 117.04(4) -2_556 . -2_556 n
Sr2 Sr1 O5 128.940(22) -2_556 . -3_556 n
O5 Sr1 O5 114.53(4) 4_554 . 5_555 n
O5 Sr1 O5 105.157(30) 4_554 . 6_554 n
O5 Sr1 O5 47.262(23) 4_554 . -1_556 n
O5 Sr1 O5 67.271(16) 4_554 . -2_556 n
O5 Sr1 O5 124.90(4) 4_554 . -3_556 n
O5 Sr1 O5 111.68(4) 5_555 . 6_554 n
O5 Sr1 O5 67.271(16) 5_555 . -1_556 n
O5 Sr1 O5 177.62(5) 5_555 . -2_556 n
O5 Sr1 O5 66.083(15) 5_555 . -3_556 n
O5 Sr1 O5 124.90(4) 6_554 . -1_556 n
O5 Sr1 O5 66.083(15) 6_554 . -2_556 n
O5 Sr1 O5 45.596(21) 6_554 . -3_556 n
O5 Sr1 O5 114.53(4) -1_556 . -2_556 n
O5 Sr1 O5 105.157(30) -1_556 . -3_556 n
O5 Sr1 O5 111.68(4) -2_556 . -3_556 n
La2 Sr2 La2 90.009(25) 1_555 . -2_565 n
La2 Sr2 La2 90.0336 1_555 . -2_566 n
La2 Sr2 SI 84.67(4) 1_555 . 2_554 n
La2 Sr2 SI 140.22(4) 1_555 . 4_664 n
La2 Sr2 SI 47.49(5) 1_555 . 6_564 n
La2 Sr2 O1 125.417(32) 1_555 . 1_555 n
La2 Sr2 O1 91.91(4) 1_555 . 3_665 n
La2 Sr2 O1 52.22(4) 1_555 . 5_565 n
La2 Sr2 O2 62.98(4) 1_555 . 2_554 n
La2 Sr2 O2 134.109(32) 1_555 . 4_664 n
La2 Sr2 O2 76.00(4) 1_555 . 6_564 n
La2 Sr2 O3 135.627(27) 1_555 . -1_665 n
La2 Sr2 O3 19.231(25) 1_555 . -3_565 n
La2 Sr2 O3 103.230(26) 1_555 . -5_555 n
La2 Sr2 Sr1 30.670(19) 1_555 . 1_565 n
La2 Sr2 Sr1 133.088(19) 1_555 . 2_554 n
La2 Sr2 Sr1 102.028(22) 1_555 . 3_555 n
La2 Sr2 Sr1 100.009(14) 1_555 . 4_664 n
La2 Sr2 Sr1 130.804(20) 1_555 . 5_665 n
La2 Sr2 Sr1 31.020(34) 1_555 . 6_564 n
La2 Sr2 Sr2 90.0001 1_555 . -2_565 n
La2 Sr2 Sr2 90.0247 1_555 . -2_566 n
La2 Sr2 La2 180.0 -2_565 . -2_566 n
La2 Sr2 SI 57.041(29) -2_565 . 2_554 n
La2 Sr2 SI 57.025(29) -2_565 . 4_664 n
La2 Sr2 SI 57.032(29) -2_565 . 6_564 n
La2 Sr2 O1 136.46(4) -2_565 . 1_555 n
La2 Sr2 O1 136.45(4) -2_565 . 3_665 n
La2 Sr2 O1 136.47(4) -2_565 . 5_565 n
La2 Sr2 O2 44.99(4) -2_565 . 2_554 n
La2 Sr2 O2 44.98(4) -2_565 . 4_664 n
La2 Sr2 O2 44.98(4) -2_565 . 6_564 n
La2 Sr2 O3 79.844(33) -2_565 . -1_665 n
La2 Sr2 O3 79.855(33) -2_565 . -3_565 n
La2 Sr2 O3 79.859(33) -2_565 . -5_555 n
La2 Sr2 Sr1 116.074(20) -2_565 . 1_565 n
La2 Sr2 Sr1 64.961(20) -2_565 . 2_554 n
La2 Sr2 Sr1 116.078(20) -2_565 . 3_555 n
La2 Sr2 Sr1 64.951(20) -2_565 . 4_664 n
La2 Sr2 Sr1 116.063(20) -2_565 . 5_665 n
La2 Sr2 Sr1 64.966(20) -2_565 . 6_564 n
La2 Sr2 Sr2 0.0 -2_565 . -2_565 n
La2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La2 Sr2 SI 122.976(29) -2_566 . 2_554 n
La2 Sr2 SI 122.960(29) -2_566 . 4_664 n
La2 Sr2 SI 122.967(29) -2_566 . 6_564 n
La2 Sr2 O1 43.54(4) -2_566 . 1_555 n
La2 Sr2 O1 43.53(4) -2_566 . 3_665 n
La2 Sr2 O1 43.55(4) -2_566 . 5_565 n
La2 Sr2 O2 135.03(4) -2_566 . 2_554 n
La2 Sr2 O2 135.02(4) -2_566 . 4_664 n
La2 Sr2 O2 135.01(4) -2_566 . 6_564 n
La2 Sr2 O3 100.139(33) -2_566 . -1_665 n
La2 Sr2 O3 100.150(33) -2_566 . -3_565 n
La2 Sr2 O3 100.154(33) -2_566 . -5_555 n
La2 Sr2 Sr1 63.931(20) -2_566 . 1_565 n
La2 Sr2 Sr1 115.043(20) -2_566 . 2_554 n
La2 Sr2 Sr1 63.935(20) -2_566 . 3_555 n
La2 Sr2 Sr1 115.033(20) -2_566 . 4_664 n
La2 Sr2 Sr1 63.920(20) -2_566 . 5_665 n
La2 Sr2 Sr1 115.048(20) -2_566 . 6_564 n
La2 Sr2 Sr2 180.0 -2_566 . -2_565 n
La2 Sr2 Sr2 0.0 -2_566 . -2_566 n
SI Sr2 SI 93.20(4) 2_554 . 4_664 n
SI Sr2 SI 93.20(4) 2_554 . 6_564 n
SI Sr2 O1 97.89(5) 2_554 . 1_555 n
SI Sr2 O1 166.23(5) 2_554 . 3_665 n
SI Sr2 O1 94.29(4) 2_554 . 5_565 n
SI Sr2 O2 28.51(4) 2_554 . 2_554 n
SI Sr2 O2 65.01(5) 2_554 . 4_664 n
SI Sr2 O2 98.42(6) 2_554 . 6_564 n
SI Sr2 O3 122.34(5) 2_554 . -1_665 n
SI Sr2 O3 92.89(4) 2_554 . -3_565 n
SI Sr2 O3 29.204(34) 2_554 . -5_555 n
SI Sr2 Sr1 111.93(4) 2_554 . 1_565 n
SI Sr2 Sr1 48.47(4) 2_554 . 2_554 n
SI Sr2 Sr1 61.953(24) 2_554 . 3_555 n
SI Sr2 Sr1 121.82(5) 2_554 . 4_664 n
SI Sr2 Sr1 144.51(4) 2_554 . 5_665 n
SI Sr2 Sr1 56.28(4) 2_554 . 6_564 n
SI Sr2 Sr2 57.033(29) 2_554 . -2_565 n
SI Sr2 Sr2 122.968(29) 2_554 . -2_566 n
SI Sr2 SI 93.20(4) 4_664 . 6_564 n
SI Sr2 O1 94.29(4) 4_664 . 1_555 n
SI Sr2 O1 97.89(5) 4_664 . 3_665 n
SI Sr2 O1 166.23(5) 4_664 . 5_565 n
SI Sr2 O2 98.42(6) 4_664 . 2_554 n
SI Sr2 O2 28.51(4) 4_664 . 4_664 n
SI Sr2 O2 65.01(5) 4_664 . 6_564 n
SI Sr2 O3 29.204(34) 4_664 . -1_665 n
SI Sr2 O3 122.34(5) 4_664 . -3_565 n
SI Sr2 O3 92.89(4) 4_664 . -5_555 n
SI Sr2 Sr1 144.51(4) 4_664 . 1_565 n
SI Sr2 Sr1 56.28(4) 4_664 . 2_554 n
SI Sr2 Sr1 111.93(4) 4_664 . 3_555 n
SI Sr2 Sr1 48.47(4) 4_664 . 4_664 n
SI Sr2 Sr1 61.953(24) 4_664 . 5_665 n
SI Sr2 Sr1 121.82(5) 4_664 . 6_564 n
SI Sr2 Sr2 57.032(29) 4_664 . -2_565 n
SI Sr2 Sr2 122.967(29) 4_664 . -2_566 n
SI Sr2 O1 166.23(5) 6_564 . 1_555 n
SI Sr2 O1 94.29(4) 6_564 . 3_665 n
SI Sr2 O1 97.89(5) 6_564 . 5_565 n
SI Sr2 O2 65.01(5) 6_564 . 2_554 n
SI Sr2 O2 98.42(6) 6_564 . 4_664 n
SI Sr2 O2 28.51(4) 6_564 . 6_564 n
SI Sr2 O3 92.89(4) 6_564 . -1_665 n
SI Sr2 O3 29.204(34) 6_564 . -3_565 n
SI Sr2 O3 122.34(5) 6_564 . -5_555 n
SI Sr2 Sr1 61.953(24) 6_564 . 1_565 n
SI Sr2 Sr1 121.82(5) 6_564 . 2_554 n
SI Sr2 Sr1 144.51(4) 6_564 . 3_555 n
SI Sr2 Sr1 56.28(4) 6_564 . 4_664 n
SI Sr2 Sr1 111.93(4) 6_564 . 5_665 n
SI Sr2 Sr1 48.47(4) 6_564 . 6_564 n
SI Sr2 Sr2 57.033(29) 6_564 . -2_565 n
SI Sr2 Sr2 122.968(29) 6_564 . -2_566 n
O1 Sr2 O1 73.25(6) 1_555 . 3_665 n
O1 Sr2 O1 73.25(6) 1_555 . 5_565 n
O1 Sr2 O2 125.02(4) 1_555 . 2_554 n
O1 Sr2 O2 93.66(4) 1_555 . 4_664 n
O1 Sr2 O2 154.23(5) 1_555 . 6_564 n
O1 Sr2 O3 88.06(5) 1_555 . -1_665 n
O1 Sr2 O3 141.15(6) 1_555 . -3_565 n
O1 Sr2 O3 68.79(5) 1_555 . -5_555 n
O1 Sr2 Sr1 106.01(5) 1_555 . 1_565 n
O1 Sr2 Sr1 71.892(30) 1_555 . 2_554 n
O1 Sr2 Sr1 40.11(4) 1_555 . 3_555 n
O1 Sr2 Sr1 122.53(4) 1_555 . 4_664 n
O1 Sr2 Sr1 62.18(4) 1_555 . 5_665 n
O1 Sr2 Sr1 133.91(4) 1_555 . 6_564 n
O1 Sr2 Sr2 136.46(4) 1_555 . -2_565 n
O1 Sr2 Sr2 43.54(4) 1_555 . -2_566 n
O1 Sr2 O1 73.25(6) 3_665 . 5_565 n
O1 Sr2 O2 154.23(5) 3_665 . 2_554 n
O1 Sr2 O2 125.02(4) 3_665 . 4_664 n
O1 Sr2 O2 93.66(4) 3_665 . 6_564 n
O1 Sr2 O3 68.79(5) 3_665 . -1_665 n
O1 Sr2 O3 88.06(5) 3_665 . -3_565 n
O1 Sr2 O3 141.15(6) 3_665 . -5_555 n
O1 Sr2 Sr1 62.18(4) 3_665 . 1_565 n
O1 Sr2 Sr1 133.91(4) 3_665 . 2_554 n
O1 Sr2 Sr1 106.01(5) 3_665 . 3_555 n
O1 Sr2 Sr1 71.892(30) 3_665 . 4_664 n
O1 Sr2 Sr1 40.11(4) 3_665 . 5_665 n
O1 Sr2 Sr1 122.53(4) 3_665 . 6_564 n
O1 Sr2 Sr2 136.46(4) 3_665 . -2_565 n
O1 Sr2 Sr2 43.54(4) 3_665 . -2_566 n
O1 Sr2 O2 93.66(4) 5_565 . 2_554 n
O1 Sr2 O2 154.23(5) 5_565 . 4_664 n
O1 Sr2 O2 125.02(4) 5_565 . 6_564 n
O1 Sr2 O3 141.15(6) 5_565 . -1_665 n
O1 Sr2 O3 68.79(5) 5_565 . -3_565 n
O1 Sr2 O3 88.06(5) 5_565 . -5_555 n
O1 Sr2 Sr1 40.11(4) 5_565 . 1_565 n
O1 Sr2 Sr1 122.53(4) 5_565 . 2_554 n
O1 Sr2 Sr1 62.18(4) 5_565 . 3_555 n
O1 Sr2 Sr1 133.91(4) 5_565 . 4_664 n
O1 Sr2 Sr1 106.01(5) 5_565 . 5_665 n
O1 Sr2 Sr1 71.893(30) 5_565 . 6_564 n
O1 Sr2 Sr2 136.46(4) 5_565 . -2_565 n
O1 Sr2 Sr2 43.54(4) 5_565 . -2_566 n
O2 Sr2 O2 75.49(6) 2_554 . 4_664 n
O2 Sr2 O2 75.49(6) 2_554 . 6_564 n
O2 Sr2 O3 124.52(6) 2_554 . -1_665 n
O2 Sr2 O3 66.34(4) 2_554 . -3_565 n
O2 Sr2 O3 57.37(4) 2_554 . -5_555 n
O2 Sr2 Sr1 93.39(4) 2_554 . 1_565 n
O2 Sr2 Sr1 71.86(4) 2_554 . 2_554 n
O2 Sr2 Sr1 86.097(31) 2_554 . 3_555 n
O2 Sr2 Sr1 105.14(5) 2_554 . 4_664 n
O2 Sr2 Sr1 160.31(5) 2_554 . 5_665 n
O2 Sr2 Sr1 32.01(4) 2_554 . 6_564 n
O2 Sr2 Sr2 44.98(4) 2_554 . -2_565 n
O2 Sr2 Sr2 135.02(4) 2_554 . -2_566 n
O2 Sr2 O2 75.49(6) 4_664 . 6_564 n
O2 Sr2 O3 57.37(4) 4_664 . -1_665 n
O2 Sr2 O3 124.52(6) 4_664 . -3_565 n
O2 Sr2 O3 66.34(4) 4_664 . -5_555 n
O2 Sr2 Sr1 160.31(5) 4_664 . 1_565 n
O2 Sr2 Sr1 32.01(4) 4_664 . 2_554 n
O2 Sr2 Sr1 93.39(4) 4_664 . 3_555 n
O2 Sr2 Sr1 71.86(4) 4_664 . 4_664 n
O2 Sr2 Sr1 86.097(31) 4_664 . 5_665 n
O2 Sr2 Sr1 105.14(5) 4_664 . 6_564 n
O2 Sr2 Sr2 44.98(4) 4_664 . -2_565 n
O2 Sr2 Sr2 135.02(4) 4_664 . -2_566 n
O2 Sr2 O3 66.34(4) 6_564 . -1_665 n
O2 Sr2 O3 57.37(4) 6_564 . -3_565 n
O2 Sr2 O3 124.52(6) 6_564 . -5_555 n
O2 Sr2 Sr1 86.097(31) 6_564 . 1_565 n
O2 Sr2 Sr1 105.14(5) 6_564 . 2_554 n
O2 Sr2 Sr1 160.31(5) 6_564 . 3_555 n
O2 Sr2 Sr1 32.01(4) 6_564 . 4_664 n
O2 Sr2 Sr1 93.39(4) 6_564 . 5_665 n
O2 Sr2 Sr1 71.86(4) 6_564 . 6_564 n
O2 Sr2 Sr2 44.98(4) 6_564 . -2_565 n
O2 Sr2 Sr2 135.02(4) 6_564 . -2_566 n
O3 Sr2 O3 116.965(20) -1_665 . -3_565 n
O3 Sr2 O3 116.965(20) -1_665 . -5_555 n
O3 Sr2 Sr1 121.239(33) -1_665 . 1_565 n
O3 Sr2 Sr1 80.792(31) -1_665 . 2_554 n
O3 Sr2 Sr1 121.362(34) -1_665 . 3_555 n
O3 Sr2 Sr1 36.808(30) -1_665 . 4_664 n
O3 Sr2 Sr1 36.219(22) -1_665 . 5_665 n
O3 Sr2 Sr1 137.47(5) -1_665 . 6_564 n
O3 Sr2 Sr2 79.853(33) -1_665 . -2_565 n
O3 Sr2 Sr2 100.147(33) -1_665 . -2_566 n
O3 Sr2 O3 116.965(20) -3_565 . -5_555 n
O3 Sr2 Sr1 36.219(22) -3_565 . 1_565 n
O3 Sr2 Sr1 137.47(5) -3_565 . 2_554 n
O3 Sr2 Sr1 121.239(33) -3_565 . 3_555 n
O3 Sr2 Sr1 80.792(31) -3_565 . 4_664 n
O3 Sr2 Sr1 121.363(34) -3_565 . 5_665 n
O3 Sr2 Sr1 36.808(30) -3_565 . 6_564 n
O3 Sr2 Sr2 79.853(33) -3_565 . -2_565 n
O3 Sr2 Sr2 100.147(33) -3_565 . -2_566 n
O3 Sr2 Sr1 121.363(34) -5_555 . 1_565 n
O3 Sr2 Sr1 36.808(30) -5_555 . 2_554 n
O3 Sr2 Sr1 36.219(22) -5_555 . 3_555 n
O3 Sr2 Sr1 137.47(5) -5_555 . 4_664 n
O3 Sr2 Sr1 121.239(33) -5_555 . 5_665 n
O3 Sr2 Sr1 80.792(31) -5_555 . 6_564 n
O3 Sr2 Sr2 79.853(33) -5_555 . -2_565 n
O3 Sr2 Sr2 100.147(33) -5_555 . -2_566 n
Sr1 Sr2 Sr1 157.965(23) 1_565 . 2_554 n
Sr1 Sr2 Sr1 102.138(25) 1_565 . 3_555 n
Sr1 Sr2 Sr1 96.147(16) 1_565 . 4_664 n
Sr1 Sr2 Sr1 102.138(25) 1_565 . 5_665 n
Sr1 Sr2 Sr1 61.578(20) 1_565 . 6_564 n
Sr1 Sr2 Sr2 116.071(20) 1_565 . -2_565 n
Sr1 Sr2 Sr2 63.929(20) 1_565 . -2_566 n
Sr1 Sr2 Sr1 61.577(20) 2_554 . 3_555 n
Sr1 Sr2 Sr1 103.372(24) 2_554 . 4_664 n
Sr1 Sr2 Sr1 96.146(16) 2_554 . 5_665 n
Sr1 Sr2 Sr1 103.372(24) 2_554 . 6_564 n
Sr1 Sr2 Sr2 64.959(20) 2_554 . -2_565 n
Sr1 Sr2 Sr2 115.041(20) 2_554 . -2_566 n
Sr1 Sr2 Sr1 157.965(23) 3_555 . 4_664 n
Sr1 Sr2 Sr1 102.138(25) 3_555 . 5_665 n
Sr1 Sr2 Sr1 96.147(16) 3_555 . 6_564 n
Sr1 Sr2 Sr2 116.071(20) 3_555 . -2_565 n
Sr1 Sr2 Sr2 63.929(20) 3_555 . -2_566 n
Sr1 Sr2 Sr1 61.577(20) 4_664 . 5_665 n
Sr1 Sr2 Sr1 103.372(24) 4_664 . 6_564 n
Sr1 Sr2 Sr2 64.959(20) 4_664 . -2_565 n
Sr1 Sr2 Sr2 115.041(20) 4_664 . -2_566 n
Sr1 Sr2 Sr1 157.965(23) 5_665 . 6_564 n
Sr1 Sr2 Sr2 116.071(20) 5_665 . -2_565 n
Sr1 Sr2 Sr2 63.929(20) 5_665 . -2_566 n
Sr1 Sr2 Sr2 64.959(20) 6_564 . -2_565 n
Sr1 Sr2 Sr2 115.041(20) 6_564 . -2_566 n
Sr2 Sr2 Sr2 180.0 -2_565 . -2_566 n
La1 O5 La1 111.890(34) 2_555 . 3_555 n
La1 O5 La1 105.81(4) 2_555 . 4_555 n
La1 O5 SI 95.36(6) 2_555 . 2_555 n
La1 O5 O3 82.59(8) 2_555 . 2_555 n
La1 O5 Sr1 0.0 2_555 . 2_555 n
La1 O5 Sr1 111.890(34) 2_555 . 3_555 n
La1 O5 Sr1 105.81(4) 2_555 . 4_555 n
La1 O5 La1 114.753(34) 3_555 . 4_555 n
La1 O5 SI 124.11(5) 3_555 . 2_555 n
La1 O5 O3 70.14(6) 3_555 . 2_555 n
La1 O5 Sr1 111.890(34) 3_555 . 2_555 n
La1 O5 Sr1 0.0 3_555 . 3_555 n
La1 O5 Sr1 114.753(34) 3_555 . 4_555 n
La1 O5 SI 102.11(6) 4_555 . 2_555 n
La1 O5 O3 166.56(8) 4_555 . 2_555 n
La1 O5 Sr1 105.81(4) 4_555 . 2_555 n
La1 O5 Sr1 114.753(34) 4_555 . 3_555 n
La1 O5 Sr1 0.0 4_555 . 4_555 n
SI O5 O3 66.16(9) 2_555 . 2_555 n
SI O5 Sr1 95.36(6) 2_555 . 2_555 n
SI O5 Sr1 124.11(5) 2_555 . 3_555 n
SI O5 Sr1 102.11(6) 2_555 . 4_555 n
O3 O5 Sr1 82.59(8) 2_555 . 2_555 n
O3 O5 Sr1 70.14(6) 2_555 . 3_555 n
O3 O5 Sr1 166.56(8) 2_555 . 4_555 n
Sr1 O5 Sr1 111.890(34) 2_555 . 3_555 n
Sr1 O5 Sr1 105.81(4) 2_555 . 4_555 n
Sr1 O5 Sr1 114.753(34) 3_555 . 4_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.0232(19) . 3_555 n
La1 La1 4.0232(19) . 5_555 n
La1 La2 4.1296(12) . 1_545 n
La1 La2 4.1302(12) . -2_556 n
La1 SI 3.2411(23) . 1_555 n
La1 SI 3.3254(24) . 5_555 n
La1 O1 2.7403(21) . 5_555 n
La1 O2 2.5075(21) . 3_655 n
La1 O3 2.6165(17) . 1_555 n
La1 O3 2.4774(11) . 6_555 n
La1 O3 2.4774(11) . -3_555 n
La1 O3 2.6165(17) . -4_556 n
La1 O4 2.3228(11) . 1_555 n
La1 Sr1 4.3067(6) . 2_554 n
La1 Sr1 4.3067(6) . 2_555 n
La1 Sr1 4.0232(19) . 3_555 n
La1 Sr1 4.0232(19) . 5_555 n
La1 Sr1 4.3067(6) . 6_554 n
La1 Sr1 4.3067(6) . 6_555 n
La1 Sr2 4.1301(12) . 1_545 n
La1 Sr2 4.2796(12) . 2_655 n
La1 Sr2 4.2796(12) . -1_665 n
La1 Sr2 4.1301(12) . -2_556 n
La1 O5 2.4790(11) . 4_554 n
La1 O5 2.63345(20) . 5_555 n
La1 O5 2.5645(11) . 6_554 n
La1 O5 2.4790(11) . -1_556 n
La1 O5 2.63345(20) . -2_556 n
La1 O5 2.5645(11) . -3_556 n
La2 La1 4.1296(12) . 1_565 n
La2 La1 4.1302(12) . 3_555 n
La2 La1 4.1305(12) . 5_665 n
La2 La2 3.6228(30) . -2_565 n
La2 La2 3.6303(30) . -2_566 n
La2 SI 3.3288(19) . 2_554 n
La2 SI 3.3293(19) . 4_664 n
La2 SI 3.3284(19) . 6_564 n
La2 O1 2.5044(15) . 1_555 n
La2 O1 2.5041(15) . 3_665 n
La2 O1 2.5037(15) . 5_565 n
La2 O2 2.5606(16) . 2_554 n
La2 O2 2.5613(16) . 4_664 n
La2 O2 2.5608(16) . 6_564 n
La2 O3 2.9058(14) . -1_665 n
La2 O3 2.9048(14) . -3_565 n
La2 O3 2.9055(14) . -5_555 n
La2 Sr1 4.1296(12) . 1_565 n
La2 Sr1 4.2800(12) . 2_554 n
La2 Sr1 4.1302(12) . 3_555 n
La2 Sr1 4.2797(12) . 4_664 n
La2 Sr1 4.1305(12) . 5_665 n
La2 Sr1 4.2792(12) . 6_564 n
La2 Sr2 0.00056 . 1_555 n
La2 Sr2 3.6228(30) . -2_565 n
La2 Sr2 3.6303(30) . -2_566 n
SI La1 3.2411(23) . 1_555 n
SI La1 3.3254(24) . 3_555 n
SI La2 3.3284(19) . 2_655 n
SI La2 3.3293(19) . -1_665 n
SI O1 1.6221(26) . 1_555 n
SI O2 1.6301(25) . 1_555 n
SI O3 1.6242(15) . 1_555 n
SI O3 1.6242(15) . -4_556 n
SI Sr1 3.2411(23) . 1_555 n
SI Sr1 3.3254(24) . 3_555 n
SI Sr1 3.6848(23) . 5_665 n
SI Sr2 3.7312(18) . 1_555 n
SI Sr2 3.3288(19) . 2_655 n
SI Sr2 3.3288(19) . -1_665 n
SI Sr2 3.7312(18) . -2_566 n
SI O5 1.7568(16) . 6_554 n
SI O5 1.7568(16) . -3_556 n
O1 La1 2.7403(21) . 3_555 n
O1 La2 2.5044(15) . 1_555 n
O1 La2 2.5041(15) . -2_566 n
O1 SI 1.6221(26) . 1_555 n
O1 Sr1 2.7403(21) . 3_555 n
O1 Sr2 2.5041(15) . 1_555 n
O1 Sr2 2.5041(15) . -2_566 n
O2 La1 2.5075(21) . 5_665 n
O2 La2 2.5608(16) . 2_655 n
O2 La2 2.5613(16) . -1_665 n
O2 SI 1.6301(25) . 1_555 n
O2 Sr1 2.5075(21) . 5_665 n
O2 Sr2 2.5609(16) . 2_655 n
O2 Sr2 2.5609(16) . -1_665 n
O3 La1 2.6165(17) . 1_555 n
O3 La1 2.4774(11) . 2_554 n
O3 La2 2.9058(14) . -1_665 n
O3 SI 1.6242(15) . 1_555 n
O3 Sr1 2.6165(17) . 1_555 n
O3 Sr1 2.4774(11) . 2_554 n
O3 Sr1 3.4064(17) . 3_555 n
O3 Sr2 2.9054(14) . -1_665 n
O3 O5 0.9463(14) . 6_554 n
O4 La1 2.3228(11) . 1_555 n
O4 La1 2.3228(11) . 3_555 n
O4 La1 2.3228(11) . 5_555 n
O4 Sr1 2.3228(11) . 1_555 n
O4 Sr1 2.3228(11) . 3_555 n
O4 Sr1 2.3228(11) . 5_555 n
Sr1 La1 4.3067(6) . 2_554 n
Sr1 La1 4.3067(6) . 2_555 n
Sr1 La1 4.0232(19) . 3_555 n
Sr1 La1 4.0232(19) . 5_555 n
Sr1 La1 4.3067(6) . 6_554 n
Sr1 La1 4.3067(6) . 6_555 n
Sr1 La2 4.1296(12) . 1_545 n
Sr1 La2 4.2792(12) . 2_655 n
Sr1 La2 4.2797(12) . -1_665 n
Sr1 La2 4.1302(12) . -2_556 n
Sr1 SI 3.2411(23) . 1_555 n
Sr1 SI 3.6848(23) . 3_655 n
Sr1 SI 3.3254(24) . 5_555 n
Sr1 O1 2.7403(21) . 5_555 n
Sr1 O2 2.5075(21) . 3_655 n
Sr1 O3 2.6165(17) . 1_555 n
Sr1 O3 3.4064(17) . 5_555 n
Sr1 O3 2.4774(11) . 6_555 n
Sr1 O3 3.4064(17) . -2_556 n
Sr1 O3 2.4774(11) . -3_555 n
Sr1 O3 2.6165(17) . -4_556 n
Sr1 O4 2.3228(11) . 1_555 n
Sr1 Sr1 4.3067(6) . 2_554 n
Sr1 Sr1 4.3067(6) . 2_555 n
Sr1 Sr1 4.0232(19) . 3_555 n
Sr1 Sr1 4.0232(19) . 5_555 n
Sr1 Sr1 4.3067(6) . 6_554 n
Sr1 Sr1 4.3067(6) . 6_555 n
Sr1 Sr2 4.1301(12) . 1_545 n
Sr1 Sr2 4.2796(12) . 2_655 n
Sr1 Sr2 4.2796(12) . -1_665 n
Sr1 Sr2 4.1301(12) . -2_556 n
Sr1 O5 2.4790(11) . 4_554 n
Sr1 O5 2.63345(20) . 5_555 n
Sr1 O5 2.5645(11) . 6_554 n
Sr1 O5 2.4790(11) . -1_556 n
Sr1 O5 2.63345(20) . -2_556 n
Sr1 O5 2.5645(11) . -3_556 n
Sr2 La1 4.1301(12) . 1_565 n
Sr2 La1 4.2796(12) . 2_554 n
Sr2 La1 4.1301(12) . 3_555 n
Sr2 La1 4.2796(12) . 4_664 n
Sr2 La1 4.1301(12) . 5_665 n
Sr2 La1 4.2796(12) . 6_564 n
Sr2 La2 0.00056 . 1_555 n
Sr2 La2 3.6228(30) . -2_565 n
Sr2 La2 3.6303(30) . -2_566 n
Sr2 SI 3.7312(18) . 1_555 n
Sr2 SI 3.3288(19) . 2_554 n
Sr2 SI 3.7312(18) . 3_665 n
Sr2 SI 3.3288(19) . 4_664 n
Sr2 SI 3.7312(18) . 5_565 n
Sr2 SI 3.3288(19) . 6_564 n
Sr2 O1 2.5041(15) . 1_555 n
Sr2 O1 2.5041(15) . 3_665 n
Sr2 O1 2.5041(15) . 5_565 n
Sr2 O2 2.5609(16) . 2_554 n
Sr2 O2 2.5609(16) . 4_664 n
Sr2 O2 2.5609(16) . 6_564 n
Sr2 O3 2.9054(14) . -1_665 n
Sr2 O3 2.9053(14) . -3_565 n
Sr2 O3 2.9053(14) . -5_555 n
Sr2 Sr1 4.1301(12) . 1_565 n
Sr2 Sr1 4.2796(12) . 2_554 n
Sr2 Sr1 4.1301(12) . 3_555 n
Sr2 Sr1 4.2796(12) . 4_664 n
Sr2 Sr1 4.1301(12) . 5_665 n
Sr2 Sr1 4.2796(12) . 6_564 n
Sr2 Sr2 3.6228(30) . -2_565 n
Sr2 Sr2 3.6303(30) . -2_566 n
O5 La1 2.5645(11) . 2_555 n
O5 La1 2.63345(20) . 3_555 n
O5 La1 2.4790(11) . 4_555 n
O5 SI 1.7568(16) . 2_555 n
O5 O3 0.9463(14) . 2_555 n
O5 Sr1 2.5645(11) . 2_555 n
O5 Sr1 2.63345(20) . 3_555 n
O5 Sr1 2.4790(11) . 4_555 n
O5 O5 1.98736(15) . -4_557 n
loop_
_pd_block_diffractogram_id
2004-06-11T10:45|LA8SR2SI6_H_01|La8Sr2Si6O26_750K|TOF
2004-06-11T10:45|LA8SR2SI6_H_02|La8Sr2Si6O26_750K|TOF
loop_
_pd_phase_block_id
2004-06-11T10:45|LA8SR2SI6_phase1|La8Sr2Si6O26_750K||
